ISRN Condensed Matter Physics

Volume 2012, Article ID 969830, 5 pages

http://dx.doi.org/10.5402/2012/969830

## Analysis of the Dielectric Constant as a Function of Temperature at Constant Electric Fields for the Smectic A-Smectic G Transition in A6

^{1}Department of Physics, Middle East Technical University, 06531 Ankara, Turkey^{2}Department of Physics, Yuzuncu Yil University, 65080 Van, Turkey

Received 25 September 2012; Accepted 10 October 2012

Academic Editors: K. Kasamatsu, R. Rossmanith, V. Stephanovich, and S. Wang

Copyright © 2012 H. Yurtseven and E. Kilit. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

The temperature dependence of the dielectric constant is studied under some fixed electric fields for the smectic G- (tilted-) smectic A (orthogonal) transition of the ferroelectric liquid crystal of compound A6. For this study, a mean field model with the quadrupole-quadrupole interactions is introduced. By fitting the inverse dielectric susceptibility from the mean field model to the experimental data from the literature, the observed behaviour of the dielectric constant is described satisfactorily for the smectic AG transition in A6. The transition temperature induced by an external electric field is also discussed for this ferroelectric compound.

#### 1. Introduction

Ferroelectric liquid crystals have been the subject of various experimental and theoretical studies [1–12]. As a function of temperature under fixed pressures or concentrations, the physical quantities such as the spontaneous polarization, tilt angle, dielectric constant, specific heat, and so forth. have been studied for their phase transitions between the smectic phases of A and C (or ) in particular. Under the electric field, some of those quantities have also been investigated and the first order or second order nature of the transitions between the smectic phases has been clarified.

Among the smectic phases, smectic C (or ) and also smectic G phases are tilted since the long axes of the molecules make an angle with the director, whereas smectic A, B, and E phases are orthogonal (). In the presence of the chiral molecules, the smectic tilted phases possess a spontaneous polarization [1]. In the chiral-racemic systems, as the spontaneous polarization increases, the ferroelectric transition temperatures are shifted. Similarly, increasing the applied electric field causes the ferroelectric transition temperatures to shift [7]. Increasing the amount of spontaneous polarization or the external electric field then changes the phase transition from a first order towards a second order in ferroelectric liquid crystals. In some ferroelectric materials, a tricritical transition [12, 13] occurs which exhibits both the features of first order and second order transitions.

The nature of the transition among the smectic phases can be investigated by considering the coupling between the order parameters (tilt angle, spontaneous polarization, orientational order parameter, etc.) in the mean field models. A bilinear coupling between the spontaneous polarization and the tilt angle ( coupling) [5, 7] and the biquadratic coupling ( coupling) [3, 4] have been considered in the mean field models mainly for the smectic AC (or ) transitions. We have also studied the AC or transitions using the biquadratic [14–18] and both the bilinear and biquadratic couplings [19, 20] in our earlier studies.

In this study, we investigate the dielectric properties of the ferroelectric liquid crystal of A6 for its smectic AG transition using our mean field model with the coupling which we have introduced previously [14]. The temperature dependence of the dielectric susceptibility is derived from our mean field model and it is fitted to the experimental data [7] for the phase transition, ransition between the tilted smectic G phase and the orthogonal smectic A phase of compound A6. This analysis of the dielectric constant (or dielectric susceptibility ) is performed for the applied electric field strengths of 0, 17, 33, 50, and kV/cm using the experimental data for A 6 [7].

Below, in Section 2, we give an outline of our mean field model regarding the dielectric susceptibility. In Section 3 our calculations and results are presented. Sections 4 and 5 give our discussion and conclusions.

#### 2. Theory

The smectic A-smectic G (AG) transition in ferroelectric liquid crystals can be studied by the mean field models where the free energy of the smectic G phase can be expanded in terms of the order parameters. Since the smectic G phase is the tilted phase such as smectic C and phases, the free energy of this phase can be expanded in terms of the tilt angle and the spontaneous polarization (order parameters) as follows:

In this mean field model (1) as we have introduced in our previous study [14], the quadrupole-quadrupole interactions () between the molecules are taken into account ( is the biquadratic coupling constant). The coefficients , , , and are independent of temperature, is the dielectric susceptibility at fixed , and is the vacuum permittivity. When is negative, smectic AG transition is of a first order, for , the tricritical AG transition occurs and this transition is of a second order when is positive.

The temperature dependence of the order parameters (tilt angle of the smectic G phase, and the spontaneous polarization P of the smectic A and G phases) and the susceptibility can be derived from the free energy (1).

By minimizing the free energy (or and ), one gets

By solving in terms of in (3) and substituting it to (1), we can express the free energy in terms of the tilt angle only, as given below:

Equations (2) and (3) give, respectively, the temperature dependence of the tilt angle of the smectic phase and the spontaneous polarization of the smectic G and A phases (when substituted (3) in (2) for ).

The temperature dependence of the dielectric susceptibility can also be derived, as stated above, according to or

Using (5) for the tilt angle susceptibility through (1), we find

The temperature dependence of the tilt angle can be obtained from the molecular field theory [21] as

Equation (8) can be used in (7) and the coefficients in the expansion of the inverse susceptibility can then be determined.

#### 3. Calculations and Results

The temperature dependence of the inverse susceptibility was analyzed according to (7) for the smectic AG transition of compound A6 using the experimental data for the dielectric constant [7]. This analysis was conducted for constant bias field strengths of 0, 17, 33, 50, and 67 kVcm^{−1} [7]. Equation (7) was fitted to the experimental data for for the field strengths studied using the variables and , as given in Table 1 within the temperature intervals in the smectic G phase () for A6. Values of the coefficients which we obtained from our analysis above in the smectic A phase () are tabulated in Table 2. In both tables, represents the experimental values [7] of the inverse susceptibility when at the critical temperature (). Our calculated (7) and the observed data for the dielectric constant are plotted as a function of temperature for the bias field strengths of 0, 17, 33, 50, and kVcm^{−1} in Figures 1, 2, 3, 4, and 5, respectively, for the smectic AG transition of compound A6.

#### 4. Discussion

The dielectric constant was calculated from the inverse dielectric susceptibility according to (7) using the experimental data [7] for both the smectic AG transition of compound A6 at various temperatures for fixed field strenghts, as shown in Figures 1, 2, 3, 4, and 5. For all the fixed electric fields by fitting (7) to the observed data [7], the fitted parameters were deduced within the temperature intervals studied (Tables 1 and 2). As seen in Figures 1, 2, 3, 4, and 5, our fits are reasonably good for the smectic AG transition as the transition temperature ) is shifted to higher values with increasing the bias field strength (Tables 1 and 2). We also estimated the temperature difference between the observed temperature and the transition temperature for the smectic G phase at zero electric field ( kVcm^{−1}) in the case of a first order smectic AG transition of compound A6. We found that for , which increases to considerably much larger values as the bias field strength increases towards kVcm^{−1}. This indicates that a first order smectic AG transition can occur at zero electric field which changes toward a second order one with increasing the field strength in A6. This is also demonstrated experimentally (Figures 1, 2, 3, 4, and 5) that the dielectric constant decreases in magnitude as the field strength increases with the transition temperature shifted. This decrease in the dielectric constant indicates most likely a second order smectic AG transition in A6. In the smectic A phase, the dielectric constant increases with decreasing temperature due to the electroclinic soft mode behaviour of the smectic A phase of chiral molecules [7]. As the electric field decreases (with decreasing temperature), the electroclinic soft mode behaviour of the smectic A phase of chiral molecules becomes more effective, which causes a sudden decrease of the dielectric constant in the tilted smectic G phase, as observed experimentally [7].

It has been reported [7] that a linear relation between the induced temperature shift and the applied field strength can be established, as studied for A6. Also, an analogy between the shift of the transition temperature induced by an external electric field and the shift induced by the spontaneous polarization can exist for ferroelectric liquid crystals [7], in particular, for compound A6. In fact, the ferroelectric transition temperatures are shifted by the increasing amount of the spontaneous polarization in the chiral-racemic systems, as pointed out previously [7]. By considering a bilinear coupling between the spontaneous polarization P and the tilt angle ( with the coupling constant C) in the mean field model, the difference in the transition temperature between the chiral compound and its racemate has been obtained [7] as

In our mean field model (1) with the biquadratic coupling ( is the coupling constant), this difference in the transition temperature can be obtained as

This can be applied to the smectic G (chiral)-smectic A (racemic) on the assumption that the spontaneous polarization refers to the smectic phase only. In order to estimate the difference in the transition temperature , we used (10) at zero electric field ( kV/cm) and we obtained the value of 0.3 K which can be compared with the value of 1.0 for the smectic AG transition of compound A6. We also calculated the difference at higher field strengths up to 67 kV/cm (Table 1). We obtained that the values of increased enormously for the smectic AG transition of A6 as the bias field strength increases. We conclude that the transition temperatures are shifted by the increasing amount of the spontaneous polarization in the case of zero electric field for the chiral-racemic systems, as studied here for the compound A6. This gives rise to a first order smectic AG transition at zero electric field for A6. Regarding the dielectric susceptibility induced by the spontaneous polarization , its temperature dependence can also be studied for ferroelectric liquid crystals, particularly for compound A6. Here, the spontaneous polarization can be defined as the total polarization of both smectic phases of A and G or for the tilted phase G only. This then requires the temperature dependence of the spontaneous polarization as we used that dependence of the tilt angle (8) from the molecular field theory. Within the biquadratic coupling (with the coupling constant D) from our mean field model (1), can be obtained as a function of temperature. In this case, the spontaneous polarization which induces the temperature shift can be considered as an internal electric field similar to the applied electric field that induces a tilt angle in ferroelectric liquid crystals.

#### 5. Conclusions

The dielectric constant was studied at various temperatures for the smectic A- smectic G transition of compound A6 in the presence of constant electric fields. The inverse dielectric susceptibility deduced from our mean field model with the biquadratic coupling, was fitted to the experimental data from the literature for the AG transition of this ferroelectric liquid crystal. It was found that the mean field model studied here describes adequately the observed behaviour of the dielectric constant as a function of temperature.

It is concluded that the smectic A-smectic G transition in A6 is of a first order at zero electric field. As the field strength increases, it changes toward a second order transition in this ferroelectric liquid crystal.

#### References

- R. B. Meyer, L. Liebert, L. Strzelecki, and P. Keller, “Ferroelectric liquid crystals: a review,”
*Journal of Physics Letters*, vol. 36, pp. 69–71, 1975. View at Google Scholar - C. C. Huang and S. C. Lien, “Effect of the smectic-A temperature range on the behavior of the smectic-A-smectic-C (or -chiral-smectic-C) transition,”
*Physical Review A*, vol. 31, pp. 2621–2627, 1985. View at Publisher · View at Google Scholar - C. C. Huang and S. Dumrongrattana, “Generalized mean-field model for the smectic A chiral-smectic-C phase transition,”
*Physical Review A*, vol. 34, no. 6, pp. 5020–5026, 1986. View at Publisher · View at Google Scholar · View at Scopus - T. Carlsson, B. Zeks, A. Levstik, C. Filipic, I. Levstik, and R. Blinc, “Generalized Landau model of ferroelectric liquid crystals,”
*Physical Review A*, vol. 36, no. 3, pp. 1484–1487, 1987. View at Publisher · View at Google Scholar · View at Scopus - C. Bahr and G. Heppke, “Influence of electric field on a first-order smectic-A-ferroelectric-smectic-C liquid-crystal phase transition: a field-induced critical point,”
*Physical Reviews A*, vol. 41, pp. 4335–4342, 1990. View at Publisher · View at Google Scholar - C. Bahr and G. Heppke, “Critical exponents of the electric-field-induced smectic-A-ferroelectric-smectic-C liquid-crystal critical point,”
*Physical Review A*, vol. 44, no. 6, pp. 3669–3672, 1991. View at Publisher · View at Google Scholar · View at Scopus - C. Bahr, G. Heppke, and B. Sabaschus, “Influence of an electric field on phase transitions in ferroelectric liquid crystals,”
*Liquid Crystals*, vol. 11, pp. 41–48, 1992. View at Publisher · View at Google Scholar - J. Zubia, M. Castro, J. A. Puertolas, J. Etxebarria, M. A. Perez Jubindo, and M. R. De la Fuente, “Character of the smectic-A-chiral-smectic-C phase transition near a chiral-nematic-smectic-A-chiral-smectic-C point,”
*Physical Review E*, vol. 48, pp. 1970–1976, 1993. View at Publisher · View at Google Scholar - K. Ema, H. Yao, A. Fukuda, Y. Takanishi, and H. Takezoe, “Non-Landau critical behavior of heat capacity at the smectic-A-smectic-${C}_{\alpha}{\hspace{0.17em}}^{\ast}$transition of the antiferroelectric liquid crystal methylheptyloxycarbonylphenyl octyloxycarbonylbiphenyl carboxylate,”
*Physical Review E*, vol. 54, pp. 4450–4453, 1996. View at Publisher · View at Google Scholar - F. Mercuri, M. Marinelli, U. Zammit, C. C. Huang, and D. Finotello, “Critical behavior of thermal parameters at the smectic-A-hexatic-B and smectic-A-smectic-C phase transitions in liquid crystals,”
*Physical Review E*, vol. 68, Article ID 051705, 10 pages, 2003. View at Publisher · View at Google Scholar - K. Denolf, B. Van Roie, G. Pitsi, and J. Thoen, “Investigation of the smectic-A-smectic-C Transition in liquid crystals by adiabatic scanning calorimetry,”
*Molecular Crystals and Liquid Crystals*, vol. 449, no. 1, pp. 47–55, 2006. View at Publisher · View at Google Scholar · View at Scopus - P. K. Mukherjee, “Tricritical behavior of the smectic-A to smectic-${\text{C}}^{\ast}$ transition,”
*Journal of Chemical Physics*, vol. 131, Article ID 074902, 7 pages, 2009. View at Publisher · View at Google Scholar - H. Y. Liu, C. C. Huang, C. Bahr, and G. Heppke, “Tricriticality near the smectic-A-smectic-C transition of a liquid-crystal compound,”
*Physical Review Letters*, vol. 61, pp. 345–348, 1988. View at Publisher · View at Google Scholar - S. Salihoǧlu, H. Yurtseven, A. Giz, D. Kayişoǧlu, and A. Konu, “The mean field model with P
^{2}*θ*^{2}coupling for the smectic A-smectic C* phase transition in liquid crystals,”*Phase Transitions*, vol. 66, no. 1–4, pp. 259–270, 1998. View at Google Scholar · View at Scopus - S. Salihoǧlu, H. Yurtseven, and B. Bumin, “Concentration dependence of polarization for the ${\text{AC}}^{\ast}$
phase transition in a binary mixture of liquid crystals,”
*International Journal of Modern Physics B*, vol. 12, pp. 2083–2090, 1998. View at Publisher · View at Google Scholar - H. Yurtseven, Y. Enginer, and S. Salihoǧlu, “Calculation of the T-X phase diagram for a mixture of liquid crystals,”
*Calphad*, vol. 24, no. 4, pp. 483–493, 2000. View at Publisher · View at Google Scholar · View at Scopus - H. Yurtseven and E. Kilit, “Temperature dependence of the polarization and tilt angle under an electric field close to the smectic AC* phase transition in a ferroelectric liquid crystal,”
*Ferroelectrics*, vol. 365, no. 1, pp. 122–129, 2008. View at Publisher · View at Google Scholar · View at Scopus - E. Kilit and H. Yurtseven, “Calculation of the dielectric constant as a function of temperature near the smectic AC* phase transition in ferroelectric liquid crystals,”
*Ferroelectrics*, vol. 365, no. 1, pp. 130–138, 2008. View at Publisher · View at Google Scholar · View at Scopus - H. Yurtseven and M. Kurt, “Spontaneous polarization and the tilt angle as a function of temperature in chiral smectic C phase of SCE9 and SCE10,”
*Balkan Physics Letters*, vol. 19, no. 191039, pp. 335–340, 2011. View at Google Scholar - H. Yurtseven and M. Kurt, “Tilt angle and the temperature shifts calculated as a function of concentration for the ${\text{AC}}^{\ast}$ phase transition in a binary mixture of liquid crystals,”
*International Journal of Modern Physics B*, vol. 25, pp. 1791–1806, 2011. View at Publisher · View at Google Scholar - M. Matsushita, “Anomalous temperature dependence of the frequency and damping constant of phonons near T
^{λ}in ammonium halides,”*Journal of Chemical Physics*, vol. 65, pp. 23–28, 1976. View at Publisher · View at Google Scholar